Plasma-induced physicochemical effects on a poly(amide)
thin-film composite membrane
Rackel Reis a*, Ludovic F. Dumée b, Andrea Merendab, John D. Orbella, Jürg A. Schützc and Mikel Dukea
Institute for Sustainability for Innovation, College of Engineering and Science, Victoria University, Hoppers Lane, Werribee, VIC 3030, Australia
Institute for Frontier Materials, Deakin University, Pigdons Road, Waurn Ponds,VIC 3216, Australia
CSIRO Manufacturing, 75 Pigdons Road, Waurn Ponds, VIC 3216, Australia
2 Abstract: Helium and water gas plasma were used to modify the surface morphology and chemistry of commercial thin film composite membranes. Such surface treatment is a convenient tool to alter performance of the membranes and subsequently reduce interactions with contaminants in solution. Plasma reactions such as etching and re-deposition resulted in surface functionalization and texturation which were correlated with membrane flux and salt rejection changes. Investigations conducted using atomic force microscopy revealed morphology alterations which were apparent as either smoother surfaces or rougher surfaces. While the smoothing was attributed to a re-deposition of polymer material, which originated most likely from vaporization of surface polymer, the roughening was a result from balanced plasma surface reactions. The beneficial etching can occur under certain conditions when helium is used in conjunction with low excitation power, which resulted in flux enhancements up to 66% (i.e. from 30 L.m-2.h-1 to 50 L.m-2.h-1) with 98 % rejection. The hydrophilicity was dramatically increased from 46.6° to as low as 8.9° after 5 min of helium plasma duration. The impact of plasma treatments have on the nascent structure was discussed in order to highlight its application as a convenient tool to functionalize the surface of thin film composite membranes.
Keywords: Plasma gas surface modification, hydrophilicity control, surface texturation,
4 1. Introduction
Thin film composite (TFC) membranes have become benchmark materials for applications 3
in nano-filtration (NF) or reverse osmosis (RO) technologies. These membranes represent a 4
performance-breakthrough with the combination of flux and selectivity in desalination 5
membranes. However, despite such phenomenal industry take-up over the last 30 years, 6
membrane damage incurred by fouling and bio-fouling still remains a key challenge [1, 2]. 7
These issues are limiting membrane performance and lifespan due to the varying water 8
quality which impacts negatively on operating costs of desalination plants. The design of 9
advanced surfaces is therefore a key to sustaining long term performance during operation 10
and to managing the adverse and unavoidable effects of fouling . Surface modifications of 11
TFC membranes are viable routes to custom design TFC membranes. Chemical routes have 12
been mainly targeted towards controlling surface hydrophobicity and roughness through 13
chemical grafting and surface coating [4-7]. Increasing the hydrophilicity of the surface will 14
reduce its affinity with organic foulants [8, 9], while reducing surface roughness can 15
significantly decrease physical adhesion of foulants and suppress solid deposition on the 16
surface [10, 11]. Although chemical grafting and surface coating were shown to reduce 17
fouling, in practice such conventional chemical techniques add to operating costs due to the 18
use of large amount of chemicals and additional treatment steps [12-14]. Novel cost-effective 19
routes are therefore sought to manufacture surface energy tunable materials with enhanced 20
Plasma chemistry is a rapidly developing technique with low environmental impact [15-22
17]. This versatile technique uses reactants in the form of gases or vapors to create distinct 23
and systematic alterations of material surface properties from short treatment times . High 24
5 suited for treating thin membrane structures due to excellent uniformity of the resulting 26
treatment and the absence of hot arcs, which can burn holes [18, 19]. Most investigations 27
involving plasma treatments have focused on modification of ultra- or micro-filtration 28
membranes [20-22] and utilized a range of reactant gases. In this regard, water (H2O) and
helium (He) plasmas are cost effective reactants for tuning the membrane surface morphology 30
and graft favorable bonding functionality for subsequent processing [23, 24]. Although some 31
benefits of plasma in membrane technology are well established, only few studies have 32
explored applying such plasma treatments to poly(amide) (PA) TFC membranes [25-27]. The 33
PA chemical structure is by nature a highly cross-linked and hierarchical material which 34
therefore several synergistic effects work in unison to achieving an exemplary desalination 35
performance. Experimental parameters (i.e. reactant gas, working pressure and excitation 36
power) are sought to be adjusted considering the specific nature of PA membrane structure in 37
order to achieve an optimal balance of surface modifications without compromising 38
performance . 39
Some plasma reactions may cause different impacts on PA structure which can be 40
beneficial if parameters are well controlled. For instance, electron-initiated reactions from RF 41
plasmas may activate and simultaneously generate free-radicals from reactants as well as 42
from polymer material of the treated substrate. Exposure to air after plasma treatment in 43
general creates more hydrophilic surfaces by incorporation of low-molecular weight oxidized 44
structures and subsequently improving anti-fouling properties [29, 30]. In addition, some 45
plasma treatments of polymeric membranes have been demonstrated to simultaneously 46
increase surface hydrophilicity and roughness which potentially contributed to flux 47
enhancement during organic fouling operation tests [25, 31, 32]. Collisions of electrons at 48
certain angles to the material surface also cause bond scissions, which remove material from 49
6 are removed from the surface, re-deposition of the same materials in vaporized phase may 51
occur [33, 34]. On the other hand, intense plasma conditions, such as high excitation power 52
and long duration, may favour some undesired reactions which can suppress functionalization 53
mechanisms. Therefore the adjustment of the excitation power is critical to controlling the 54
extent of etching on the surface. Such mechanisms are governed by UV emissions present in 55
RF plasma, and therefore the treated material’s inherent UV absorption capacity may strongly 56
facilitate such reactions . For example, UV absorption in PA occurs mainly in the vicinity 57
of 300 nm wavelength . Intense UV absorption may lead to excessive re-deposition, 58
cross-linking and branching of macromolecules which can potentially penetrate as far as 200 59
nm into the PA layer. The resultant process may reduce surface area  and create 60
membrane resistance, a similar issue also found in surface coating modifications [4, 13, 38] 61
which can also impact on membrane flux [15, 39]. 62
In this work, for the first time, commercial TFC membranes were treated with pure He and 63
H2O gas plasma for a broad range of excitation power and exposure durations. The plasma
powers were therefore chosen to cover a broad range of potential plasma excitation energies, 65
as well as different levels of emitted UV light, from the plasma glows. The investigation also 66
sought to evaluate their impact on the material’s morphology, surface energy and 67
microstructure, being parameters known to affect membrane performance. This study gives 68
in-depth insights into membrane performance associated with plasma surface reactions 69
contrasted by two divergent gas reactants. The modified membranes were characterized and 70
potential practical improvements for desalination performance were discussed. 71
7 2. Experimental Section
2.1 Reagents and materials 74
BW30 TFC membranes were purchased from Dow Filmtec Corp. (IMCD limited 75
Australia). The TFC RO membrane is a multilayer material composed of an extremely thin 76
active (~100-200 nm) and semi-dense layer of PA. This layer is deposited on top of a thick 77
porous support substrate (e.g. poly(sulfone) (PSf)) coated on to a nonwoven (e.g. poly(ester) 78
(PES)) fabric structure . Membranes were conditioned prior to plasma processing by 79
immersing them in deionized (DI) water for 5 hours, dried in air and then rinsed with ethanol 80
prior to permeation. This procedure represents the common activation process for new 81
membranes of this type. 82
2.2 Plasma treatments 83
Plasma treatments were performed using a low pressure plasma system from Diener 84
Plasma Surface Technology, model Pico-RF-PC and operating in the high frequency band at 85
13.56 MHz. Reactants were water H2O and He, which were injected into a 7.7 L
steel chamber at a constant pressure of 0.2 mbar and exposed to either 10 W or 80 W 87
excitation power for a duration of 1, 2 or 5 min. Immediately after plasma treatment the 88
membranes were purged in nitrogen for 20 seconds in order to avoid oxidation in air and 89
better preserve the chemical modification. 90
2.3 Characterization techniques 91
2.3.1 Scanning Electron Micrographs (SEM) 92
SEM images were obtained from a Quanta dual beam Gallium (Ga) Focus Ion Beam (FIB) 93
8 analysis. Images were collected at 20 keV acceleration voltage with a working distance of 10 95
2.3.2 Atomic Force Microscopy (AFM) 97
Atomic force microscopy (AFM) analysis was performed in tapping mode using a Bruker 98
model Nanoscope V with multimode scanning capability and equipped with a microscope 99
camera 10xA Nikon series 110422 to monitor the scanning area. The resonance frequency 100
and force constant of the cantilever probe was 300 kHz (±100 kHz) and 40 N/m, respectively. 101
Data was collected using Nanoscope 8.4 software, providing a scan window size of 7 µm. 102
Images were subsequently evaluated using Gwyddion.36 data analysis software. The 103
accuracy of plotted data sets was within a 95% confidence interval of the true value. 104
2.3.3 Contact angle 105
Contact angle measurements were performed with a Biolin Scientific goniometer to map 106
differences in hydrophobicity across the membrane surface. Contact angle measurements 107
were performed 1 hour after plasma treatment. Each test involves applying 4 μL of de-ionized 108
water in the form of drops in three different spots on the membrane surface. Images were 109
acquired 5 seconds after application of the water drop and contact angles were calculated by 110
fitting the image of the drops using the Young-Laplace algorithm from the optical tensiometer 111
software. Plotted data lies within the 95% confidence interval of the true value. 112
2.3.4 Attenuated Total Reflection-Fourier Transform Infrared Spectroscopy (ATR-113
Analysis of surface functional groups created by the plasma treatments was performed 115
using a Perkin Elmer infrared spectrometer, model Frontier with KBr beam splitter and 116
9 cm-1, 8 spectra were averaged at resolution of 4 cm-1 and analyzed with OPUS 7.2 software 118
from Bruker Corporation. 119
2.3.5 X ray photoelectron spectroscopy (XPS) 120
X-ray photoelectron spectroscopy (XPS) was utilized for surface and interface 121
characterization. XPS was performed using a Thermo Scientific™ K-Alpha+™ X-ray 122
photoelectron spectrometer. The photon energy was 1253.6 eV, line width 0.7 eV and Mg 123
Kalpha hv=486.7 nm filament. A quantitative elemental composition of the modified PA was
provided for a surface depth of 1–5 nm and detection limit of 0.1% of the bulk material. The 125
peak position was calibrated using the C1s peak at 284.6 eV. 126
2.4 Membrane performance 127
Salt rejection and water permeation performance were tested with a laboratory-scale cross-128
flow filtration system model CF042 from Sterlitech Corp., WA, USA. The circulating feed 129
stream contained 2,000 mg/L of sodium chloride (NaCl) from Sigma Aldrich (99% purity) at 130
25°C. The effective membrane area was 42 cm2 and the trans-membrane pressure was 131
monitored and maintained at the target working pressure of 15 bar within +/- 2% accuracy. 132
The circulating permeate flow at the outlet was collected after 2 h and salt rejection 133
conductivity measured immediately on completion of the test. Salt concentration was 134
determined using an electrical conductivity meter (Hach HQ40d) and permeate mass was 135
measured using a balance with a resolution of 0.001 grams. Data acquisition software was 136
used to record the permeate flux for a 1 min interval. Each desalination test was replicated 137
twice and error bars of about 7% were obtained after considering the estimated standard error 138
of the mean values. 139
10 Salt rejection R (%) was calculated according to:
𝑅 = 1 − (𝐶𝐶𝑝
𝑓) × 100% (1)
where Cp and Cf are measured conductivities of the collected permeate and initial feed (in
µS/cm), respectively, which represent the corresponding salt concentrations, assuming that 145
the conversion between conductivity and concentration is linear within corresponding 146
concentration ranges. Total permeate flux Jw(L.m-2.h-1) was calculated by:
𝐽𝑤 = 𝑉
𝐴×𝑡 (2) 148
where V is volume of the permeate (L), A is effective membrane area (m2) and t is time in 149
hours over which the volume V was collected. 150
3. Results and Discussion 151
3.1 The impact of plasma treatments on membrane performance 152
The impact of various plasma treatment conditions on membrane performance, including 153
the total flux and salt rejection, were investigated first. The total water flux and salt rejection 154
of various treated membranes, as measured in a cross-flow set up, is displayed in Figure 1 as 155
a function of the nature of etchant gas, excitation power and process duration. The use of 156
NaCl solution is a standard procedure to investigate the integrity of the PA layer after plasma 157
modification. Although other salts may have been selected, the small kinetic diameter of Na+ 158
ions as well as the single charge on both ions is pertinent properties for the testing of the 159
integrity of the material. Flux for the untreated reference membrane was 30 L.m-2.h-1, and is 160
indicated as the first bar on each of the sub-figures. NaCl salt rejection was 97%. These levels 161
of flux and rejection are typical for state of the art brackish water TFC membranes provided 162
11 The flux through the membranes after H2O plasma treatment at 0.2 mbar and 10 W was
found to be statistically similar to that of the reference membranes at any plasma treatment 165
duration with no significant loss in salt rejection, as shown in Figure 1. At 80 W, however, 166
the flux was significantly reduced after 2 min of plasma treatment, while rejection remained 167
unaffected in comparison to the control membrane. At the longer treatment time of 5 min, a 168
sharp loss in salt rejection was observed, declining to 84%. Conversely, the permeation of He 169
plasma treated membranes at 10 W showed systematic flux increases as a function of the 170
exposure duration while simultaneously exhibiting slight rejection loss. The flux for the 1 and 171
2 min treated samples improved by up to 17%, and up to 66% for the 5 min treated 172
membrane. At 80 W of plasma excitation power the flux of He plasma treated membranes 173
declined, while rejection remained approximately constant at 98.8 ± 0.5 %. 174
Resultant processes produced vastly different outcomes as a function of both exposure 175
duration and excitation power. In order to understand the effect of plasma treatments on the 176
modified surface, further physico-chemical characterization of modified membrane surface is 177
required to explain the observed increases in permeation. 178
3.2 Membrane characterization 179
Competitive plasma surface reactions arise from the etching processes, which can lead to 180
differing degrees of surface functionalization and roughening . If plasma conditions are 181
intensified, a net re-deposition of vaporized materials can result in the surface becoming 182
smoother by cross-linking and free volume densification . 183
Etching promotes bond scission processes  and simultaneously, chemical bond 184
reformation may lead to texturation and roughness changes on the membrane surface. Bond 185
reformation may be confined to the outermost PA layer and present as temporary surface 186
12 further stimulated by UV light from the plasma, the process can result in internal PA cross-188
linking [33, 34]. Chemical effects from etching, in conjunction with re-deposited, vaporized 189
materials, may also occur as a result of high excitation power and long exposure time, which 190
leads to reduced surface roughness. Oxidative gases can especially promote aromatic rings 191
scissions [43, 44] and lead to severe PA degradation due to potential polymer backbone bond 192
scissions . 193
The interplay of these competing effects is believed to be at the core of experimental 194
observations made and is discussed in the following in terms of physical and chemical 195
changes occurring on the membrane. 196
3.2.1 Morphology characterization of the plasma modified membranes 197
Initial investigations of morphology changes were performed by acquiring SEM images of 198
the membrane surfaces as a function of the treatment conditions. Figure 2a shows the SEM of 199
the control membrane . As shown in Figure 3, the surface of the H2O treated membranes
was significantly smoothed with increasing treatment duration, with the effect intensified for 201
higher excitation power. In contrast, the topographical SEM analysis for He plasma in Figure 202
4 shows that modified membranes at 10 W were slightly smoothed for short plasma 203
treatments, while roughening occurred for a treatment time of 5 min. The same effect was 204
also found at 80 W. 205
In order to confirm topology variations found by SEM, the average roughness (Ra) for 206
the modified membranes was measured by AFM and compared with a control membrane with 207
Ra of 63 nm (Figure 2b). As shown in Figure 5 and Table S1, H2O treated membranes at 10
W showed reduced Ra from 63 nm (control) down to 43 ± 2.6 nm after only 1 min of plasma 209
treatment. Beyond 1 min, the roughness values increased back up to Ra 57 ± 5.0 nm between 210
13 reduced down to 57 ± 2.5 nm at 1 min, to 36 ± 2.2 nm at 2 min, and then 47 ± 4.3 nm at 5 212
min. Previous studies on CO2 plasma treatment of poly(ether sulfone) (PES) membrane also
demonstrated that smoothed morphologies were achieved for the treated surfaces . The 214
SEMs showed that between 1 to 5 min of plasma treatment pores were gradually reduced in 215
diameter and progressively disappeared. However, beyond 5 min, the pore size started to 216
increase again and to reappear across the surface. The alterations of pore diameters were 217
attributed to etching and re-depositions on the surface. Interestingly, the etching rate was 218
found to be largely depending on the power density than the re-deposition rate for this 219
Here, the smoothing was not consistent with He plasma treatment, as shown in Figure 221
6 and Table S2. At 10 W there was a progressive roughening trend, similar to that reported 222
for the SEM analysis. For shorter treatment durations, between 1 and 2 min, the roughness 223
was slightly reduced to 60 ± 0.5 nm and 58 ± 1.2 nm. However, a significant roughening 224
effect was observed with longer plasma treatment, with Ra increasing to 70 ± 1.5 nm at 5 min 225
which is in good agreement with previously reported study . A similar roughening effect 226
was observed with helium plasma (25 W) treatment on PES membranes. Significantly 227
increased roughness values were measured from 11 nm (control) to 39 nm after 30 s of 228
plasma treatment duration. Although these roughening mechanisms may be attributed to 229
fragments of re-deposited materials, the exact mechanisms involved were not conclusive to 230
date . He plasma at 80 W, however, showed a smoothing trend, stronger than observed 231
for water plasma, with Ra reduced to around 40 ± 2.7 nm for all durations which therefore 232
may be attributed to re-deposition of molecular fragments of removed materials. 233
Increased resistance to water flux through the PA layer promoted by H2O plasma (i.e.
decreased water fluxes observed in Figure 1) may be due to a potential densification of the 235
14 plasma at 80 W. In this regard, the use of He at 10 W appeared to provide successful etching 237
with balanced plasma conditions  resulting in increased surface area, which contributed to 238
the flux enhancement shown in Figure 1. Material hydrophobicity also plays a role in altered 239
membrane performance [51, 52] and further chemical analysis is needed. 240
3.2.2 Chemical characterization of the plasma modified membranes 241
Investigation of the chemical functional group changes across the membranes was 242
performed by ATR-FTIR analysis. Variations in absorbance from studied frequencies 243
(described in Table S3) showed potential degradation and functionalization of aromatic rings 244
in the polymer backbone. 245
The analysis of the FTIR spectra (Figure 7) for H2O plasma modified membranes showed
that absorbance decreased with the broadening of the band at 3330 cm-1, corresponding to N-247
H and OH groups stretching vibration, for both 10 W and 80 W. This effect is an indication of 248
chemical degradation commonly found with oxygen containing plasmas . Although a 249
broadening peak was observed at both power intensities, possible etching at 80 W suggests an 250
intensified physical erosive behavior, confirmed with significant salt rejection loss with only 251
84 % after 5 min of treatment (Figure 1).The bands at 1663, 1609 and 1541 cm-1 generally 252
showed similar absorbance patterns for both 10 and 80 W. However, a functionalization 253
reaction at longer exposure time (5 min at 80 W, Figure 7) showed a new carbonyl band 254
around 1734 cm-1, attributed to post-plasma reactions with unreacted radicals or peroxide 255
radical . These absorbance alterations suggest an ageing process due to a large amount of 256
free-radicals with high excitation power, which can potentially contribute to a hydrophilicity 257
For He plasma modified membranes, the bands at 3330 cm-1 (Figure 8) increased in 259
15 min duration may indicate functionalization in the amide groups with OH groups . At 80 261
W, the band shifted to 3400 cm-1, which suggests changes to the neighboring hydrogen 262
bonding [53, 54]. The bands at 1663, 1609 and 1541 cm-1 followed similar absorbance 263
patterns for the He plasma at 10W. However, stronger absorbance variations were found at 80 264
W, which may indicate a potential increase in the etching effect. Therefore, functionalization 265
reactions were more likely to be found with He plasma at low power. 266
In order to investigate functionalization at the molecular level, an XPS elemental survey 267
analyzed the N/C and O/C ratio. The O/C ratio for H2O (Table S4) plasma varied slightly,
ranging between 0.2 and 0.4. The O/C ratio for H2O plasma (Table S5) was stable, and may
be related to the nature of PA. As the material already has nitrogen and oxygen functional 270
groups in the polymer structure, the incorporation of more of them via plasma treatment will 271
make them very much less visible than with other polymers treated in similar conditions . 272
The N/C ratio increased from 0.03 (control)  to 0.1 for both He and H2O plasmas, with
increased excitation power and duration. The nitrogen source is potentially N2+ metastable
species in the gaseous mixture from residual nitrogen, introduced as purge gas after plasma 275
treatment, since minimal nitrogen concentrations (> 1%) can easily react with aromatic 276
structures due to the inherent electron delocalization from aromatics. Therefore, the 277
increased ratio suggests strong correlations with functionalization, promoted by plasma 278
activation. Details from potential reaction mechanisms were not conclusive. 279
Functionalization was also investigated using contact angle analysis. Resultant 280
hydrophilicity or hydrophilicity of the outer modified layers can be achieved with 281
morphology  or chemical changes . As expected, the contact angle for all plasma 282
modified membranes was significantly reduced (Figure 9). He plasma treatment resulted in 283
consistently lower contact angles for all duration times and power levels compared with H2O.
16 Competitive processes between functionalization and re-deposition have led to 286
hydrophilicity and morphological alteration, which were correlated with roughness and 287
contact angle. The increased wettability found for membranes treated with H2O plasma at 10
W showed that with 1 min of plasma treatment the contact angle was well correlated with the 289
decreased surface roughness. After 1 min the resultant hydrophilicity is potentially correlated 290
with the chemical nature of the modified surface, potentially caused by re-deposition of 291
removed materials. Conversely, He plasma at 10 W showed that decreased contact angles 292
were more correlated with reduced roughness for 1 and 2 min durations, with stronger 293
functionalization processes occurring after 2 min. The optimum experimental conditions 294
obtained with He plasma at 5 min duration at 10W suggest a potential treatment for designing 295
membranes with more resistance to protein adhesion (fouling), since hydrophilicity is an 296
important index for antifouling properties of membranes [3, 26, 47, 60, 61]. Intense re-297
deposition (Figure 9) was more significant at 80 W, where hydrophilicity was better 298
correlated with morphology once roughness was significantly reduced, as well as contact 299
angle. On the other hand, despite the resultant rough surface morphology of the He plasma 300
treated sample and particularly for the 5 min and 10 W treated sample, a significantly reduced 301
contact angle (10.1 ± 2.0o) was measured compared to the control membrane (46.6 ± 3.0o). 302
This lower contact angle may be predominantly related to the re-deposition of etched material 303
on the surface of the membrane. These reconfigured etched materials are very likely to be 304
hydrophilic given the nature and chemistry of the initial membrane material.Therefore, the 305
rougher aspect combined with the functionalization achieved with low contact angles, have 306
preferred water transport for modified membranes. These results are in agreement with other 307
surface modification techniques, such as plasma polymerization and chemical grafting of 308
hydrophilic moieties that increased roughness upon surface hydrophilization with reduced 309
17 4. Conclusions
The impact of H2O and He plasma on PA surfaces have been investigated. He plasma
increased membrane flux by 66% with a 5 min treatment at the lower excitation power of 10 313
W, without significant loss in salt rejection. At higher power for both gases there was reduced 314
membrane flux, and for H2O plasma there were physical changes on the surface leading to
loss of salt rejection with exposure time. Surface smoothing has been shown to increase the 316
mass transfer resistance of membranes, while significant roughening was achieved with He at 317
10 W, 5 min, suggesting that plasma under these conditions provided well balanced reactions. 318
Inert gas plasma has been shown to be beneficial in modifying PA material structure. Future 319
work with other inert gases could be explored towards surface tuning and anti-fouling 320
The authors would like to acknowledge a PhD stipend and project funding from the 326
Collaborative Research Network initiative of the Australian Department of Industry. RR 327
acknowledges the postgraduate top up scholarship from the National Centre of Excellence in 328
Desalination Australia, funded by the Australian Government through the National Urban 329
Water and Desalination Plan. Dr. Ludovic Dumée’s Alfred Deakin Post-Doctoral Fellowship 330
Figure 1: Membrane flux and salt rejection measured after 2 h of testing with 2,000 ppm of 334
NaCl in water at 15 bar feed pressure after plasma modification at 0.2 mbar. 335
Figure 2: a) SEM image of control membrane and b) AFM analysis of control membrane 339
with Ra 63 nm. 340
Figure 3: SEM images from H2O plasma modified membranes.
24 Figure 7: FTIR analysis from H2O plasma modified membranes: on the top, analysis of N-H
25 Figure 8: FTIR analysis from He plasma modified membranes: on the top, analysis of N-H and O-H bands at 3330 cm-1for modified membranes at 10 W and 80 W; on the bottom, analysis of amide bands from1663 to 1541 cm-1 for modified membranes at 10 W and 80 W
27 Supplement Material
Table S1: Influence of H2O plasma on surface roughness and flux
Power density Membranes Roughness (nm)
- Control 63.0 30.0
H2O 1min 43.0 24.0
H2O 2min 58.0 27.0
H2O 5 min 57.0 26.0
H2O 1min 57.0 10.0
H2O 2min 36.0 14.0
H2O 5 min 47.0 21.0
Power density Membranes Roughness (nm)
He 1 min 60.0 34.0
He 2 min 58.0 35.0
He 5 min 70.0 49.8
He 1 min 40.0 10.0
He 2 min 42.0 15.0
He 5 min 40.0 20.7
28 FTIR frequency (cm-1) Description
3330 N-H groups and O-H groups stretching vibration
1663 Amide I band: stretching vibration from the C=O and C-C-N deformation vibration  1609 Aromatic amide N–H deformation vibration or
C=C ring stretching vibration 
1541 Amide II band: N-H in-plane bending and N-C stretching vibration of a –CO-NH- 
(at%) (at%) N (at%) O N/C O/C
Control 77.5 2.2 20.3 0.03 0.3
H2O 1 min 80.6 3.3 16.1 0.04 0.2
H2O 2 min 84.9 2.1 13.0 0.02 0.4
H2O 5 min 72.5 8.1 19.4 0.1 0.3
H2O 1 min 79.1 5.0 15.9 0.1 0.2
H2O 2 min 74.6 6.9 18.5 0.1 0.2
H2O 5 min 72.6 8.8 18.6 0.1 0.2
Table S4:Elemental XPS analysis from H2O plasma with increasing N/C ratio 
Table S5:Elemental XPS analysis from He plasma with increasing N/C ratio  Power
Control 77.5 2.2 20.3 0.03 0.3
He 2 min 73.3 6.7 20.0 0.1 0.3
1. Shenvi, S.S., A.M. Isloor, and A.F. Ismail, A review on RO membrane technology: Developments and challenges. Desalination, 2015. 368: p. 10-26.
2. Cadotte, J.E., Petersen, R.J., Larson, R.E., Erickson, E.E. , A New Thin-film Composite Seawater Reverse Osmosis Membrane. Desalination, 1980. 32: p. 25-31. 3. Lee, K.P., T.C. Arnot, and D. Mattia, A review of reverse osmosis membrane
materials for desalination development to date and future potential. Journal of Membrane Science, 2011. 370(1–2): p. 1-22.
4. Yu, S., et al., Surface modification of thin-film composite polyamide reverse osmosis membranes by coating n-isopropylacrylamide-co-acrylic acid copolymers for improved membrane properties. J. Membr. Sci., 2011. 371: p. 293-306.
5. Rana, D. and T. Matsuura, Surface modifications for antifouling membranes. Chemical Reviews (Washington, DC, U. S.), 2010. 110(4): p. 2448-2471.
6. Kang, G., et al., A novel method of surface modification on thin-film composite reverse osmosis membrane by grafting poly(ethylene glycol). Polymer, 2007. 48(5): p. 1165-1170.
7. Cheng, Q., et al., Surface modification of a commercial thin-film composite polyamide reverse osmosis membrane through graft polymerization of N-isopropylacrylamide followed by acrylic acid. J. Membr. Sci., 2013. 447: p. 236-245.
8. Kang, G.-d. and Y.-m. Cao, Development of antifouling reverseosmosis membranes for water treatment: a review. Water Research, 2012. 46(3): p. 584-600.
9. Kulkarni, A., D. Mukherjee, and W.N. Gill, Flux enhancement by hydrophilization of thin film composite reverse osmosis membranes. Journal of Membrane Science 1996. 114(1): p. 39-50.
10. Vrijenhoek, E.M., M. Elimelech, and S. Hong, Influence of membrane surface properties on initial rate of colloidal fouling of reverse osmosis and nanofiltration membranes. Journal of Membrane Science 2001. 188(1): p. 115-128.
11. Tang, C.Y., Y.-N. Kwon, and J.O. Leckie, Probing the nano and micro-scales of reverse osmosis membranes - a comprehensive characterization of physiochemical properties of uncoated and coated membranes by XPS, TEM, ATR-FTIR, and streaming potential measurements. Journal of Membrane Science, 2007. 287(1): p. 146-156.
12. Pan, K., H. Gu, and B. Cao, Interfacially polymerized thin-film composite membrane on UV-induced surface hydrophilic-modified polypropylene support for nanofiltration. Polym. Bull. (Heidelberg, Ger.), 2014. 71(2): p. 415-431.
13. Wu, D., et al., Modification of aromatic polyamide thin-film composite reverse osmosis membranes by surface coating of thermo-responsive copolymers P(NIPAM-co-Am). I: Preparation and characterization. J. Membr. Sci., 2010. 352(1-2): p. 76-85.
31 15. Fridman, A., Plasma Chemistry. 2008, Cambridge University New York.
16. Borcia, C., G. Borcia, and N. Dumitrascu, Relating plasma surface modification to polymer characteristics. Appl. Phys. A: Mater. Sci. Process., 2008. 90(3): p. 507-515. 17. Sadiqali Cheruthazhekatt, M.C., Pavel Slavicek, Josef Havel, Gas plasmas and
plasma modified materials in medicine. J. Appl. Biomed., 2010. 8: p. 55-66.
18. Pethrick, R.A., Plasma surface modification of polymers: relevance to adhesion. Polymer International. Vol. 39. 1996: John Wiley & Sons. 79-79.
19. Shenton, M.J. and G.C. Stevens, Surface modification of polymer surfaces: atmospheric plasma versus vacuum plasma treatments. Journal of Physics D: Applied Physics, 2001. 34(18): p. 2761.
20. Juang, R.-S., C. Huang, and C.-L. Hsieh, Surface modification of PVDF ultrafiltration membranes by remote argon/methane gas mixture plasma for fouling reduction. J. Taiwan Inst. Chem. Eng., 2014. 45(5): p. 2176-2186.
21. Khulbe, K.C., C. Feng, and T. Matsuura, The art of surface modification of synthetic polymeric membranes. Journal of Applied Polymer Science, 2010. 115(2): p. 855-895.
22. Nidal Hilal, M.K., Chris J.Wright, Membrane Modification Technology and Applications. Vol. 1. 2012, Florida, U.S: CRC Press.
23. Tompkins, B.D. and E.R. Fisher, Evaluation of polymer hydrophobic recovery behavior following H2O plasma processing. Journal of Applied Polymer Science,
24. Mariana, G., et al., Surface cross linking and functionalization of poly(ethylene terephthalate) in a helium discharge. Plasma Sources Sci. Technol., 1997. 6(1): p. 8. 25. Kim, E.-S. and B. Deng, Effect of NH3 plasma on thin film composite membrane:
relationship of membrane and plasma properties. Membrane Water Treatment, 2013. 4(2): p. 109-126.
26. Kim, E.-S., Q. Yu, and B. Deng, Plasma Surface Modification of Nanofiltration (NF) Thin-Film Composite (TFC) Membranes to Improve Anti Organic Fouling. Appl. Surf. Sci., 2011. 257(23): p. 9863-9871.
27. Reis, R., et al., Amine enrichment of thin film composite membranes via low pressure plasma polymerization for antimicrobial adhesion. ACS Appl Mater Interfaces, 2015. 7(27): p. 14644-53.
28. Saxena, N., et al., Flux enhancement by argon–oxygen plasma treatment of polyethersulfone membranes. Separation and Purification Technology, 2009. 70(2): p. 160-165.
29. Arefi-Khonsari, F. and M. Tatoulian, Plasma Processing of Polymers by a Low-Frequency Discharge with Asymmetrical Configuration of Electrodes, in Advanced Plasma Technology. 2008, Wiley-VCH Verlag GmbH & Co. KGaA. p. 137-174. 30. Tompkins, B.D., J.M. Dennison, and E.R. Fisher, H2O plasma modification of
32 31. u, L., et al., Surface hydrophilic modification of RO membranes by plasma polymerization for low organic fouling. Journal of Membrane Science, 2011. 369(1– 2): p. 420-428.
32. Švorčík, V., et al., Modification of surface properties of high and low density polyethylene by Ar plasma discharge. Polymer Degradation Stability, 2006. 91(6): p. 1219-1225.
33. Barton, D., et al., An In Situ Comparison between VUV photon and ion energy fluxes to polymer surfaces immersed in an rf plasma. The Journal of Physical Chemistry B, 2000. 104(30): p. 7150-7153.
34. Friedrich, J., Interaction between Plasma and Polymers, in The Plasma Chemistry of Polymer Surfaces. 2012, Wiley-VCH Verlag GmbH & Co. KGaA. p. 11-33.
35. Chan, C.M., T.M. Ko, and H. Hiraoka, Polymer surface modification by plasmas and photons. Surface Science Reports, 1996. 24(1–2): p. 1-54.
36. Liquori, A.M., A. Mele, and V. Carelli, Ultraviolet absorption spectra of polyamides. J. Polym. Sci., 1953. 10(5): p. 510-512.
37. Švorčík, V., et al., Ablation and water etching of poly(ethylene) modified by argon plasma. Polym. Degrad. Stab., 2007. 92(9): p. 1645-1649.
38. Louie, J.S., et al., Effects of polyether–polyamide block copolymer coating on performance and fouling of reverse osmosis membranes. J. Membr. Sci., 2006. 280(1–2): p. 762-770.
39. Gancarz, I., G. Poźniak, and M. Bryjak, Modification of polysulfone membranes 1. CO2 plasma treatment. Eur. Polym. J., 1999. 35(8): p. 1419-1428.
40. Filmtec, D. Reverse osmosis membranes, technical manual: http://msdssearch.dow.com/PublishedLiteratureDOWCOM/dh_0042/0901b80380042 dd2.pdf?filepath=liquidseps/pdfs/noreg/609-02002.pdf (accessed in July 2015). 41. Friedrich, J., The plasma chemistry of polymer surfaces advanced techniques for
surface design. 2012: Weinheim : Wiley-VCH.
42. Blais, P., D.J. Carlsson, and D.M. Wiles, Surface changes during polypropylene photo-oxidation: A study by infrared spectroscopy and electron microscopy. Journal of Polymer Science Part A-1: Polymer Chemistry, 1972. 10(4): p. 1077-1092.
43. Prohaska, G.W., E.D. Johnson, and J.F. Evans, Preparation and characterization of plasma-polymerized styrene thin films. Journal of Polymer Science: Polymer Chemistry Edition, 1984. 22(11): p. 2953-2972.
44. Friedrich, J., Bulk, Ablative, and Side Reactions, in The Plasma Chemistry of Polymer Surfaces. 2012, Wiley-VCH Verlag GmbH & Co. KGaA. p. 145-195.
45. Pawde, S.M. and K. Deshmukh, Surface characterization of air plasma treated poly vinylidene fluoride and poly methyl methacrylate films. Polym. Eng. Sci., 2009. 49(4): p. 808-818.
33 47. Wavhal, D.S. and E.R. Fisher, Modification of porous poly(ether sulfone) membranes by low-temperature CO2-plasma treatment. Journal of Polymer Science Part B: Polymer Physics, 2002. 40(21): p. 2473-2488.
48. Chen, H. and G. Belfort, Surface modification of poly(ether sulfone) ultrafiltration membranes by low-temperature plasma-induced graft polymerization. Journal of Applied Polymer Science, 1999. 72(13): p. 1699-1711.
49. Fujioka, T., et al., Rejection of small and uncharged chemicals of emerging concern by reverse osmosis membranes: The role of free volume space within the active skin layer. Separation and Purification Technology, 2013. 116: p. 426-432.
50. Kim, S.H., S.-Y. Kwak, and T. Suzuki, Positron Annihilation Spectroscopic Evidence to Demonstrate the Flux-Enhancement Mechanism in Morphology-Controlled Thin-Film-Composite (TFC) Membrane. Environmental Science & Technology, 2005. 39(6): p. 1764-1770.
51. Al-Jeshi, S. and A. Neville, An investigation into the relationship between flux and roughness on RO membranes using scanning probe microscopy. Desalination, 2006. 189(1–3): p. 221-228.
52. Hirose, M., H. Ito, and Y. Kamiyama, Effect of skin layer surface structures on the flux behaviour of RO membranes. J. Membr. Sci. , 1996. 121(2): p. 209-215.
53. Coates, J., Interpretation of Infrared Spectra, A Practical Approach, in Encyclopedia of Analytical Chemistry. 2006, John Wiley & Sons, Ltd.
54. Tse, K.C.C., F.M.F. Ng, and K.N. Yu, Photo-degradation of PADC by UV radiation at various wavelengths. Polymer Degradation and Stability, 2006. 91(10): p. 2380-2388.
55. Yasuda, H., et al., ESCA study of polymer surfaces treated by plasma. J. Polym. Sci., Part A: Polym. Chem., 1977. 15(4): p. 991-1019.
56. Tang, C.Y., Y.-N. Kwon, and J.O. Leckie, Effect of membrane chemistry and coating layer on physiochemical properties of thin-film composite polyamide RO and NF membranes: I. FTIR and XPS characterization of polyamide and coating layer chemistry. Desalination, 2009. 242(1–3): p. 149-167.
57. Dufour, T., et al., Chemical mechanisms inducing a dc current measured in the flowing post-discharge of an RF He-O 2 plasma torch. Plasma Sources Sci. Technol., 2012. 21(4).
58. Kubiak, K., et al., Wettability Versus Roughness of Engineering Surfaces. Wear, 2011. 271(3): p. 523-528.
59. Holmes-Farley, S.R., C.D. Bain, and G.M. Whitesides, Wetting of functionalized polyethylene film having ionizable organic acids and bases at the polymer-water interface: relations between functional group polarity, extent of ionization, and contact angle with water. Langmuir, 1988. 4(4): p. 921-937.
34 61. Wavhal, D.S. and E.R. Fisher, Hydrophilic modification of polyethersulfone membranes by low temperature plasma-induced graft polymerization. Journal of Membrane Science, 2002. 209(1): p. 255-269.
62. Kang, G., et al., Surface Modification of a Commercial Thin Film Composite Polyamide Reverse Osmosis Membrane by Carbodiimide-Induced Grafting with Poly(ethylene glycol) Derivatives. Desalination, 2011. 275(1–3): p. 252-259.